# granulometria.xls

June 12, 2019 | Author: mikiworld | Category: Units Of Measurement, Nature

#### Description

MALLA

PESO (gr)

% RET

% RET ACUM

% Q PASA

75

3"

0

0

0

100

62.5

2 1/2"

0

0

0

100

50

2"

0

0

0

100

37.5

1 1/2"

0

0

0

100

25

1”

442.50

3.705564628

3.705564628

96.29443537

19

¾"

7468.50

62.54239417

66.2479588

33.7520412

12.5 9.5

½”

3794.50

3/8”

98.02369887 99.37612528

1.976301135 0.623874723

6 .3

1/4"

161.50 41.00

31.77574007 1.352426412 0.343340451

99.71946573

0.280534271

FONDO

33.50

0.280534271

100

0

TOTAL

11941.5

100

Modulo de finura

7.66

T.M.N.=

25

MALLA

PESO (gr)

% RET

% RET ACUM

% Q PASA

4.75

Nº 4

17

3.40000

3.40000

96.60000

2.36

Nº 8

64

12.80000

16.20000

83.80000

1.18

Nº 16

118.5

23.70000

39.90000

60.10000

0 .6

Nº 30

110.5

22.10000

62.00000

38.00000

0 .3

Nº 50

92

18.40000

80.40000

19.60000

0.15

Nº 100

62.5

12.50000

92.90000

7.10000

0.075

FONDO

35.5

7.10000

100.00000

0.00000

TOTAL

5 00

100

Modulo de finura

2.95

T.M.N.=

4.75

Se resolvera la siguiente ecuacion conociendo conociendo el modulo de finura del Agregado Global (MFA) * (A) + (MFP) * (P) = MFAGLOBAL  A + P = 1 TIPO DE DE MA MAQUINA

MFAGLOBAL

5.4-5.6

MIXER

5.2-5.4

BOMBEO

5-5.1

A=

0.50

P=

0.50

0.50 MALLA

% Ret. Grueso

Peso Ret. Grueso

0.50 % Ret. Fino

Peso Ret. Fino

3"

0

0.00

0.00

0.00

2 1/2"

0

0.00

0.00

0.00

2"

0

0.00

0.00

0.00

1 1/2"

0

0.00

0.00

0.00

1”

0

0.00

0.00

0.00

¾"

0.21

0.10

0.00

0.00

½”

33.28

16.63

0.00

0.00

3/8”

32.33

16.15

0.00

0.00

1/4"

27.17

13.57

0.00

0.00

Nº 4

0

0.00

2.70

1.35

Nº 8

0

0.00

17.00

8.51

Nº 16

0

0.00

20.30

10.16

Nº 30

0

0.00

20.70

10.36

Nº 50

0

0.00

20.80

10.41

Nº 100

0

0.00

12.30

6.16

FONDO

7.01

3.50

6.20

3.10

TOTAL

1 00

49.95

100.00

50.05

TAMIZ malla nº 4"

ASTM 1 tamaño mm

%que pasa

100.000 90.000 75.000 63.000 50.000 37.500 25.000 19.000 12.500 9.500 4.750 2.360 1.180

3 1/2" 3" 2 1/2" 2" 1 1/2" 1" 3/4" 1/2" 3/8" Nº4 Nº8 Nº16

90mm a 3

100 90 57.5 25 12.5 0 0 0 0 0 0 0 0

100 100 80 60 37.5 15 10 5 0 0 0 0 0

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20 0

0. 1

1

10 Tamaño mm

TAMIZ malla nº 3/8"

PORCENTA GRUESO C

tamaño mm

9.500

100

100

Nº4

4.750

95

100

Nº8

2.360

80

100

Nº16

1.180

50

100

Nº30

0.600

25

100

Nº50

0.300

10

70

Nº100

0.150

2

12

120.00000    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100.00000 80.00000 60.00000 40.00000 20.00000 0.00000

0.1

1

10

Tamaño mm

a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

0.1

33.50

6.3

100 41.00 90 161.50 80    ) 70 3794.50    %    ( 60 7468.50   a   s 50   a 40   p 442.50   e 30   u 0   q 20   o 10 0    d   a 0    l 0   u   m 100.00   u 0   c

6.3

A

6.3 9.5 12.5 19 25 37.5 50

10.00

62.5

0

1.00 Diámetro de las partículas (mm)

75

100 80    )    %    ( 60   a   s   a 40   p   e   u   q 20   o    d 0   a    l   u 100.00   m   u   c    A

35.5

0.075

62.5

0.075

92

0.15

110.5

0.3

118.5

0.6

64

1.18

17

2.36

0

4.75

10.00

1.00 Diámetro de las partículas (mm)

5.3

MFAGLOBAL=

DIAMETRO 75 62.5 50 37.5

Este valor se elijira

MALLA

% Ret.

% Ret. Acumulado % Que Pasa

3"

0.00

0.00

100.00

2 1/2"

0.00

0.00

100.00

2"

0.00

0.00

100.00

1 1/2"

0.00

0.00

100.00

25

1”

0.00

0.00

100.00

19

¾"

0.10

0.10

99.90

12.5

½”

16.63

16.73

83.27

9.5

3/8”

16.15

32.88

67.12

6.3

1/4"

13.57

46.45

53.55

4.75

Nº 4

1.35

47.80

52.20

2.36

Nº 8

8.51

56.31

43.69

1.18

Nº 16

10.16

66.47

33.53

0.6

Nº 30

10.36

76.83

23.17

0.3

Nº 50

10.41

87.24

12.76

0.15

Nº 100

6.16

93.40

6.60

0.075

FONDO

6.60

100.00

0.00

TOTAL

100.00

Modulo de Finura

5.30

RUESO .5mm

[3 1/2" a 1 1/2"]

ASTM 2

%retenido acumulado 0 10 42.5 75 87.5 100 100 100 100 100 100 100 100

63mm a 37.5mm

%que pasa

0 0 20 40 62.5 85 90 95 100 100 100 100 100

[2 1/2" a 1 1/2"]

100 100 90 35 0 0 0 0 0 0 0 0 0

100 100 100 70 15 10 5 0 0 0 0 0 0

0 0 10 65 100 100 100 100 100 100 100 100 100

0 0 0 30 85 90 95 100 100 100 100 100 100

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100

1000

100 80 60 40 20 0

0.1

1

10 Tamaño mm

FINO

100

1000

E QUE PASA MEDIO M

FINO F

100

100

100

100

85

100

89

100

65

100

80

100

45

100

70

100

25

80

55

100

5

48

5

70

0

12

0

12

120.00000    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100.00000 80.00000 60.00000 40.00000 20.00000 0.00000

0.1

1 Tamaño mm

120.00000 100.00000 80.00000 60.00000 40.00000 20.00000 0.00000 1 Tamaño mm

10

10

ASTM 57

Balde de 1/2 pie cubico Peso de balde Peso de balde + piedra suelta Peso de balde + piedra comp

0.10

0.01

TAMIZ MALLA NRO 3'' 2 1/2'' 2'' 1 1/2'' 1'' 3/4'' 1/2'' 3/8'' 1/4'' FONDO SUMA

0.10

0.01

CUR

100 90

80    )    %    (   a   s   a   p   e   u   q   o    d   a    l   u   m   u   c    A

70 60 50 40 30 20 10 0 100.00

10.00

ASTM 3

50mm a 25mm

[2" a 1"]

ASTM

%que pasa

100 100 100 100 90 35 0 0 0 0 0 0 0

100 100 100 100 100 70 15 10 5 0 0 0 0

0 0 0 0 10 65 100 100 100 100 100 100 100

0 0 0 0 0 30 85 90 95 100 100 100 100

%que pasa

100 100 100 100 95 65 35 22.5 10 5 0 0 0

100 100 100 100 100 85 70 50 30 17.5 5 0 0

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

120

100

a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

80 60 40 20 0

0.1

10 Tamaño mm

1000

100 80 60 40 20 0

0.1

HUSO GRANULOMETRICO

HUSO Malla

31.500 16.000

I 100 62

II 100 80

8.000 4.000 2.000 1.000 0.250

38 23 14 8 2

62 47 37 28 8

tamaño mm

120.00    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100.00 80.00 60.00 40.00 20.00 0.00

0.1

1

120.00    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100.00 80.00 60.00 40.00 20.00 0.00

0.1

1

120.00    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100.00 80.00 60.00 40.00 20.00 0.00

0.1

1

33.45

:

12 kg PESO RETENIDO EN LA MALLA 0.00

(%)PORCENTAJE RETENIDO 0.00

0.00

0.00

0.00

0.00

0.00

0.00

0.00

0.00

0.00

442.50

26.03

26.03

7468.50

439.32

0.67

3794.50

223.21

223.88

161.50

9.50

233.38

41.00

2.41

235.79

33.50

1.97

1.00

11941.5

702.4411765

MODULO DE FINURA

1.00

0.10

Diámetro de las partículas (mm)

57

50mm a 4.75mm

[2" a Nº4]

%que

0 0 0 0 5 35 65 77.5 90 95 100 100 100

0 0 0 0 0 15 30 50 70 82.5 95 100 100

100 100 100 100 100 90 20 0 0 0 0 0 0

a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

1

10 Tamaño mm

100

1000

0.1

100 89 80 70 55 5 0 GRANULOMETRICO DEL AGREGADO GLOBAL ORCENTAJE QUE PASA

III 100 89 77 65 53 42 15

10

100

1000

100

1000

Tamaño mm

10 Tamaño mm

10 Tamaño mm

100

1000

Peso de piedra suelta Kg

Kg Kg

(%)ACUMULADO QUE PASA 100.00 100.00 100.00 100.00 73.97 99.33 -123.88 -133.38 -135.79 99.00 ?

0.01

ASTM 4

37.5mm a 19mm

[1 1/2" a 3/4"]

pasa

100 100 100 100 100 100 55 15 10 5 0 0 0

%que

0 0 0 0 0 10 80 100 100 100 100 100 100

0 0 0 0 0 0 45 85 90 95 100 100 100

120 100 80 60 40 20 0 1

10 Tamaño mm

100

1000

100 100 100 100 100 95 65 35 22.5 10 0 0 0

F

100 100 100 100 100 70 12

ASTM 467

37.5mm a 4.75mm

[1 1/2" a Nº4]

pasa

100 100 100 100 100 100 85 70 50 30 5 0 0

%

0 0 0 0 0 5 35 65 77.5 90 100 100 100

0 0 0 0 0 0 15 30 50 70 95 100 100

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20 0

0.1

1

10 Tamaño mm

100

1000

100 100 100 100 100 100 90 20 0 0 0 0 0

ASTM 5

25mm a 12.5mm

[1" a 1/2"]

que pasa

100 100 100 100 100 100 100 55 10 5 0 0 0

%qu

0 0 0 0 0 0 10 80 100 100 100 100 100

0 0 0 0 0 0 0 45 90 95 100 100 100

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20 0

0.1

1

10 Tamaño mm

100

1000

100 100 100 100 100 100 90 40 10 0 0 0 0

ASTM 56

25mm a 9.5mm

[1" a 3/4]

ASTM 57

pasa

100 100 100 100 100 100 100 85 40 15 5 0 0

%que pasa

0 0 0 0 0 0 10 60 90 100 100 100 100

0 0 0 0 0 0 0 15 60 85 95 100 100

100 100 100 100 100 100 95 60 25 12.5 0 0 0

100 100 100 100 100 100 100 80 60 35 10 5 0

120

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20

100 80 60 40 20 0

0 0.1

25mm

1

10 Tamaño mm

100

1000

0.1

4.75mm

[1" a Nº4]

ASTM 6

%retenido acumulado 0 0 0 0 0 0 5 40 75 87.5 100 100 100

0 0 0 0 0 0 0 20 40 65 90 95 100

19mm a 9.5mm

[3/4" a 3/8"]

%retenido a

%que pasa

100 100 100 100 100 100 100 90 20 0 0 0 0

100 100 100 100 100 100 100 100 55 15 5 0 0

0 0 0 0 0 0 0 10 80 100 100 100 100

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20 0

10 amaño mm

1000

0.1

1

10 Tamaño mm

100

ASTM 67

19mm a 4.75mm

%que pasa

0 0 0 0 0 0 0 0 45 85 95 100 100

[3/4" a Nº4]

100 100 100 100 100 100 100 90 55 20 0 0 0

100 100 100 100 100 100 100 100 77.5 55 10 5 0

0 0 0 0 0 0 0 10 45 80 100 100 100

0 0 0 0 0 0 0 0 22.5 45 90 95 100

120    a    s    a    p    e    u    q    e    j    a    t    n    e    c    r    o    P    %

100 80 60 40 20 0

1000

0.1

1

10 Tamaño mm

100

1000

ASTM 7

12.5mm a 4.75mm

ASTM 8

%que pasa

100 100 100 100 100 100 100 100 90 40 0 0 0

[1/2" a Nº4]

100 100 100 100 100 100 100 100 100 70 15 5 0

0 0 0 0 0 0 0 0 10 60 100 100 100

9.5mm a

%que pasa

0 0 0 0 0 0 0 0 0 30 85 95 100

100 100 100 100 100 100 100 100 100 85 10 0 0

100 100 100 100 100 100 100 100 100 100 30 10 5

120

120

a 100    s    a    p    e 80    u    q    e    j 60    a    t    n    e 40    c    r    o    P    % 20

a 100    s    a    p    e 80    u    q    e    j 60    a    t    n    e 40    c    r    o    P    % 20

0

0 1

10

100 Tamaño mm

1000

0

2.36mm

[3/4" a Nº8]

%retenido acumulado 0 0 0 0 0 0 0 0 0 15 90 100 100

50 Tamaño mm

0 0 0 0 0 0 0 0 0 0 70 90 95

100

CURVA GRANULOM

100 80    )    %    ( 60   a   s   a 40   p   e   u 20   q   o    d   a 0    l   u   m 100.00   u   c    A

10.00 Diámet CURVA GRANULOM

100 80

)    %    ( 60   a   s   a 40   p   e   u 20   q   o    d 0   a    l   u 100.00   m   u   c    A

10.00 Diámet CURVA GRANULOM

100 90 80    ) 70    %    ( 60   a   s   a 50   p   e   u 40   q   o    d 30   a    l   u 20   m   u   c 10    A

0 100.00

10.00 Diáme

COMPARACION GRAN GLOBAL CON HUSO I    a    s    a    p    e    u    q

120.00 100.00 80.00

e    j    a    t    n    e    c    r    o    P    %

60.00 40.00 20.00 0.00 0.1

1

10 Tamaño mm

100

1000

1.00

0.10

0.01

0.10

0.01

o de las partículas (mm) TRICA DEL AGREGADO GRUESO

1.00 o de las partículas (mm) ETRICA DEL AGREGADO GLOBAL

1.00

0.10

0.01

ro de las partículas (mm)

COMPARACION GRAN GLOBAL CON HUSO II

a

120.00

COMPARACI

a    s    a

1 1

s    a    p    e    u    q    e    j    a    t    n    e    c    r    o 0.1    P    %

100.00 80.00 60.00 40.00 20.00 0.00 1

10 Tamaño mm

100

1000

e    u    q    e    j    a    t    n    e    c    r    o    P    %

0.1

N GRAN GLOBAL CON HUSO III

20.00 00.00